In covalent bonding stable electron configurations are assumed by the sharing of electrons between adjacent atoms. Two atoms that are covalently bonded will each contribute at least one electron to the bond, and the shared electrons may be considered to belong to both atoms. Covalent bonding is schematically illustrated in Figure 2.10 for a molecule of methane (CH4). The carbon atom has four valence
electrons, whereas each of the four hydrogen atoms has a single valence electron. Each hydrogen atom can acquire a helium electron configuration (two 1s valence electrons) when the carbon atom shares with it one electron. The carbon now has four additional shared electrons, one from each hydrogen, for a total of eight valence
Table 2.3 Bonding Energies and Melting Temperatures for
Bonding Energy Melting
kJ/mol eV/Atom, Temperature Bonding Type Substance (kcal/mol) Ion, Molecule (ⴗC )
Ionic NaCl 640 (153) 3.3 801 MgO 1000 (239) 5.2 2800 Covalent Si 450 (108) 4.7 1410 C (diamond) 713 (170) 7.4 ⬎3550 Hg 68 (16) 0.7 ⫺39 Metallic Al 324 (77) 3.4 660 Fe 406 (97) 4.2 1538 W 849 (203) 8.8 3410 van der Waals Ar 7.7 (1.8) 0.08 ⫺189 Cl2 31 (7.4) 0.32 ⫺101 Hydrogen NH3 35 (8.4) 0.36 ⫺78 H2O 51 (12.2) 0.52 0 Shared electron from hydrogen Shared electron from carbon H H C H H
FIGURE2.10 Schematic representation of
covalent bonding in a molecule of methane (CH4).
2.6 Primary Interatomic Bonds ● 23
electrons, and the electron structure of neon. The covalent bond is directional; that is, it is between specific atoms and may exist only in the direction between one atom and another that participates in the electron sharing.
Many nonmetallic elemental molecules (H2, Cl2, F2, etc.) as well as molecules
containing dissimilar atoms, such as CH4, H2O, HNO3, and HF, are covalently
bonded. Furthermore, this type of bonding is found in elemental solids such as diamond (carbon), silicon, and germanium and other solid compounds composed of elements that are located on the right-hand side of the periodic table, such as gallium arsenide (GaAs), indium antimonide (InSb), and silicon carbide (SiC).
The number of covalent bonds that is possible for a particular atom is deter- mined by the number of valence electrons. For N⬘valence electrons, an atom can covalently bond with at most 8⫺N⬘other atoms. For example, N⬘ ⫽7 for chlorine, and 8⫺N⬘ ⫽1, which means that one Cl atom can bond to only one other atom, as in Cl2. Similarly, for carbon, N⬘ ⫽ 4, and each carbon atom has 8 ⫺ 4, or
four, electrons to share. Diamond is simply the three-dimensional interconnecting structure wherein each carbon atom covalently bonds with four other carbon atoms. This arrangement is represented in Figure 3.16.
Covalent bonds may be very strong, as in diamond, which is very hard and has a very high melting temperature,⬎3550⬚C (6400⬚F), or they may be very weak, as with bismuth, which melts at about 270⬚C (518⬚F). Bonding energies and melting temperatures for a few covalently bonded materials are presented in Table 2.3. Polymeric materials typify this bond, the basic molecular structure being a long chain of carbon atoms that are covalently bonded together with two of their available four bonds per atom. The remaining two bonds normally are shared with other atoms, which also covalently bond. Polymeric molecular structures are discussed in detail in Chapter 4.
It is possible to have interatomic bonds that are partially ionic and partially covalent, and, in fact, very few compounds exhibit pure ionic or covalent bonding. For a compound, the degree of either bond type depends on the relative positions of the constituent atoms in the periodic table (Figure 2.6) or the difference in their electronegativities (Figure 2.7). The wider the separation (both horizontally— relative to Group IVA—and vertically) from the lower left to the upper-right-hand corner (i.e., the greater the difference in electronegativity), the more ionic the bond. Conversely, the closer the atoms are together (i.e., the smaller the difference in electronegativity), the greater the degree of covalency. The percent ionic character of a bond between elements A and B (A being the most electronegative) may be approximated by the expression
% ionic character⫽兵1⫺ exp[⫺(0.25)(XA⫺XB)2]其⫻ 100 (2.10)
where XAand XBare the electronegativities for the respective elements.
Metallic bonding, the final primary bonding type, is found in metals and their alloys.
A relatively simple model has been proposed that very nearly approximates the bonding scheme. Metallic materials have one, two, or at most, three valence elec- trons. With this model, these valence electrons are not bound to any particular atom in the solid and are more or less free to drift throughout the entire metal. They may be thought of as belonging to the metal as a whole, or forming a ‘‘sea of electrons’’ or an ‘‘electron cloud.’’ The remaining nonvalence electrons and atomic nuclei form what are called ion cores, which possess a net positive charge equal in magnitude to the total valence electron charge per atom. Figure 2.11 is a
24 ● Chapter 2 / Atomic Structure and Interatomic Bonding
schematic illustration of metallic bonding. The free electrons shield the positively charged ion cores from mutually repulsive electrostatic forces, which they would otherwise exert upon one another; consequently the metallic bond is nondirectional in character. In addition, these free electrons act as a ‘‘glue’’ to hold the ion cores together. Bonding energies and melting temperatures for several metals are listed in Table 2.3. Bonding may be weak or strong; energies range from 68 kJ/mol (0.7 eV/atom) for mercury to 850 kJ/mol (8.8 eV/atom) for tungsten. Their respective melting temperatures are⫺39 and 3410⬚C (⫺38 and 6170⬚F).
Metallic bonding is found for Group IA and IIA elements in the periodic table, and, in fact, for all elemental metals.
Some general behaviors of the various material types (i.e., metals, ceramics, polymers) may be explained by bonding type. For example, metals are good conduc- tors of both electricity and heat, as a consequence of their free electrons (see Sections 12.5, 12.6,兵and 17.4其). By way of contrast, ionically and covalently bonded materials are typically electrical and thermal insulators, due to the absence of large numbers of free electrons.
Furthermore, in Section 8.5 we note that at room temperature, most metals and their alloys fail in a ductile manner; that is, fracture occurs after the materials have experienced significant degrees of permanent deformation. This behavior is explained in terms of deformation mechanism (Section 8.3), which is implicitly related to the characteristics of the metallic bond. Conversely, at room temperature ionically bonded materials are intrinsically brittle as a consequence of the electrically charged nature of their component ions (see Section 8.15).
Secondary, van der Waals, or physical bonds are weak in comparison to the primary or chemical ones; bonding energies are typically on the order of only 10 kJ/mol (0.1 eV/atom). Secondary bonding exists between virtually all atoms or molecules, but its presence may be obscured if any of the three primary bonding types is present. Secondary bonding is evidenced for the inert gases, which have stable
+ ⫺ + ⫺ + ⫺ + + ⫺ + ⫺ + ⫺ + + ⫺ + ⫺ + ⫺ + + + + + Ion cores
Sea of valence electrons
FIGURE2.11 Schematic illustration of
2.7 Secondary Bonding or Van der Waals Bonding ● 25
electron structures, and, in addition, between molecules in molecular structures that are covalently bonded.
Secondary bonding forces arise from atomic or molecular dipoles. In essence, an electric dipole exists whenever there is some separation of positive and negative portions of an atom or molecule. The bonding results from the coulombic attraction between the positive end of one dipole and the negative region of an adjacent one, as indicated in Figure 2.12. Dipole interactions occur between induced dipoles, between induced dipoles and polar molecules (which have permanent dipoles), and between polar molecules. Hydrogen bonding, a special type of secondary bonding, is found to exist between some molecules that have hydrogen as one of the constit- uents. These bonding mechanisms are now discussed briefly.